Circular polarization in a non-magnetic resonant tunneling device
© dos Santos et al; licensee Springer. 2011
Received: 13 September 2010
Accepted: 25 January 2011
Published: 25 January 2011
We have investigated the polarization-resolved photoluminescence (PL) in an asymmetric n-type GaAs/AlAs/GaAlAs resonant tunneling diode under magnetic field parallel to the tunnel current. The quantum well (QW) PL presents strong circular polarization (values up to -70% at 19 T). The optical emission from GaAs contact layers shows evidence of highly spin-polarized two-dimensional electron and hole gases which affects the spin polarization of carriers in the QW. However, the circular polarization degree in the QW also depends on various other parameters, including the g-factors of the different layers, the density of carriers along the structure, and the Zeeman and Rashba effects.
The understanding of the physics governing the dynamics of spin-polarized carriers in semiconductor structures is a fundamental issue for the development of new spintronic devices. In the past years, several systems have been proposed for spin-based devices, including magnetic metal/semiconductor junctions, all metallic devices, and all semiconductor systems [1–10]. However, the change of the polarization requires the use of an applied external magnetic field to change the contact magnetization. For some device applications, it would be interesting to have devices where the spin character of the injected or detected electrons could be voltage selected. One possible approach to achieve this goal is based on resonant tunneling diodes (RTDs) because the spin character of the carriers in the structure could be voltage controlled [11–15].
In this work, we have investigated the polarization-resolved photoluminescence (PL) from different regions in a non-magnetic asymmetric n-type RTD with a GaAs quantum well (QW) and AlAs and AlGaAs barriers. This asymmetry was used to increase the accumulation of charge of carriers in the QW. Under applied bias, electrons tunnel through the double-barrier structure creating a two-dimensional electron gas (2DEG) in the QW and at the accumulation layers next to the barriers which densities and g-factors are bias voltage dependent. The spin-dependent tunneling of carriers was studied by analyzing the current-voltage characteristics (I(V)) and the right (σ+) and left (σ-) circular polarized PL from the contact layers and from the QW under magnetic fields up to 19 T. High magnetic fields were used in order to increase the spin-related effects in our non-magnetic RTD. The main goal of the present work is to investigate the fundamental physics of spin-related effects in our structures, but this is an essential step for analyzing the feasibility of using RTD structures for spintronic devices in the future.
We have observed small oscillations on the QW circular polarization degree as a function of the applied voltage with values up to -70% at 19 T. We have also observed optical emission from spin-polarized 2DEG and two-dimensional hole gas (2DHG) in the GaAs contact layers next to emitter and collector barriers. Under applied bias voltage, polarized carriers from contact layer tunnel through the double-barrier region and contribute to the spin polarization of carriers in the QW. The circular polarization of the QW emission seems to depend on various other points, including the g-factors of the different layers, the spin-polarization of injected carriers from the contact region, the density of carriers along the structure, and the Rashba and Zeeman effects.
Our device was grown by molecular beam epitaxy on a n + (001) GaAs substrate. The double-barrier region consists of 2 μm n-GaAs (1 × 1018 cm-3), 0.1 μm n-GaAs (1 × 1017 cm-3), 51 Å undoped GaAs spacer, 40 Å AlAs barrier, 50.9 Å GaAs QW, 42 Å Al0.4Ga0.6As barrier, 51 Å GaAs spacer, 0.1 μm n-GaAs (1 × 1017 cm-3), and 0.51 μm n-GaAs (1 × 1018 cm-3). Circular mesas of 400 μm diameter were processed with annular AuGe contacts which allow optical measurements. Micro-PL measurements were performed at 4 K under magnetic fields up 19 T parallel to the tunnel current. The measurements were performed by using optical fibers and a Si CCD system coupled with a Jobin-Yvon spectrometer. A linearly polarized beam from an Ar+ laser (all lines) was used for optical excitation. Therefore, photogenerated carriers in the structure do not present any preferential spin polarization. The right (σ+) and left (σ-) circularly polarized emissions were selected with appropriate optics and by reversing the current in the electromagnet.
Under applied bias, photo-created holes can tunnel (resonantly or non-resonantly) and recombine with tunneling electrons into the QW and contact layers. The PL intensity from the QW is, in first approximation, proportional to the product of hole and electron densities. Therefore, it is very sensitive to the variation of charge density in the QW which can be voltage controlled in resonant tunneling devices. As a consequence, the PL intensity is, in general, correlated to the I(V) characteristic curves. In our experimental conditions, the optical emission from the QW was not detected under zero bias voltage, which indicates that the optical generation of carriers inside the QW is negligible.
Figure 1b shows typical polarization-resolved PL spectra for our device at 0.52 V. In general, the GaAs contact emission includes several bands: the free-exciton (FE) transition from the undoped space-layer, the recombination between photogenerated holes and donor related electrons from the n-doped GaAs layers (D-H), and the indirect recombination between free holes (electrons) and confined electrons (holes) localized at the 2DEG (or 2DHG) formed at the accumulation layer next to the barriers (2DEG-h or 2DHG-e emissions). In particular, only the 2DEG-h space-indirect emission was recently observed for p-i-n RTDs . However, its voltage dependence and its contribution to the spin polarization of carriers in the QW were not investigated. In order to have more information about the contribution of both spin-polarized 2DEG and 2DHG to circular polarization degree of the QW emission, we performed a detailed measurement of the PL emissions as a function of the applied bias in our resonant tunneling structure.
Figure 1c shows the current voltage characteristics curve (I(V)) under dark and under light excitation at zero magnetic field. We have observed one electron resonant peak at V 1 = 0.32 V which was associated with the resonant tunneling through the first confined electron state e1 in the QW. Under light excitation, this resonant peak (e1) shifts to lower voltages. This shift is an evidence that the hole charge density has increased in the double-barrier region. Actually, an increase of the hole density in the QW reduces the total charge accumulated in the QW and shifts the electron resonant peak to lower voltages. The hole density at the accumulation layer also increases when we increase the applied voltage which results in the formation of a 2DHG next to the collector barrier (at the surface side, as illustrated in Figure 1a). As mentioned earlier, the energy position of confined levels in the 2DHG and QW can be voltage controlled. The hole resonant tunneling condition can be obtained by the alignment between the confined levels at the accumulation layer (2DHG) and QW. This effect is evidenced by the observation of an additional structure at 0.125 V in the I(V) curve under light excitation which was associated with the first heavy hole resonance (hh1) (Figure 1c). This additional structure hh1 is better defined under magnetic field (Figure 1d). In addition, we have observed that photocurrent under low voltages is markedly larger than the electron current in the dark, which indicates that the holes actually become the effective majority carrier under this voltage condition.
Figure 2d-f presents the voltage dependence of the PL from the GaAs contact layers. As discussed earlier, this emission includes several bands: the FE transition, the recombination between photogenerated holes and donor-related electrons (broad band) and the voltage-dependent peaks which were associated with the indirect recombination between free electrons (holes) and the 2DHG (2DEG) at the accumulation layers (Figure 1a). The 2DHG-e emission is observed for low bias voltage, before the onset of hole resonant tunneling condition while the peak attributed to the 2DEG-h recombination is only observed under applied magnetic field, for bias voltages in the range of 0.1 < V < 0.5 V (Figure 2e,f).
We observed that an increase the applied bias results in a decrease of 2DHG-e emission intensity and in an increase of FE emission intensity. When we increase the applied voltage, photogenerated holes are swept away from the 2DHG by the increased electric field, and excitons are predominantly formed in the GaAs layer reducing the intensity of this 2DHG-e indirect transition. At hole resonant tunneling condition, holes tunnel through the QW which results in a reduction of hole density accumulated in the 2DHG which can also reduce the PL intensity of 2DHG-e emission. An abrupt transfer of FE emission to 2D electron - 3D hole emission was previously observed with increasing magnetic field (perpendicular to the 2DEG plane) for integer and fractional filling factors (ν < 2) on high quality modulation doped GaAs/AlGaAs heterojunction (HJ) [16–19]. Actually, it was observed that for filling factors ν < 2 the FE PL intensity decreases and a new lower energy PL line abruptly appears and gain intensity at expense of the exciton PL. This abrupt transfer was explained by a phenomenological dynamical model which considers an exciton dissociation near the magnetized 2DEG. In this model, the dissociation rate depends on exciton dynamics in two well potentials that is formed by FE near the HJ interface and 3D hole interacting with the 2DEG . Our system is, however, more complex than a simple HJ structure. A variation of the applied voltage in the RTD results not only in strong variations of the carrier densities at the accumulation layers, and therefore variation of the filling factor of the 2D gases in the structure, but it also directly alters the electric field along the structure, and consequently, the potential profile V(z) at the accumulation layers. A complete analysis of the results requires detailed calculations, but we point out some general points which are consistent with our interpretation. The 2DHG-e peak is only observed before the onset of hole-tunneling, as for larger voltages the relatively small reservoir of photo-created holes (2DHG) accumulated at the top barrier interface must be mainly depleted. The 2DEG-h transition is observed at the electron resonant tunneling condition. Its intensity (Figure 2f) initially increases with bias voltage, which is consistent with increasing densities of tunneling holes and electrons accumulated at the 2DEG, but it shows some reduction at the e1 resonance peak, as at this condition the density of the 2DEG should be somehow reduced. At about 0.45 V, when the I(V) characteristic curve shows an abrupt current reduction, the 2DEG-h shows an abrupt increase of intensity which is consistent with a sudden increase of electron density accumulated at the 2DEG. For large voltages (>0.5 V), the 2DEG-h emission tends to vanish, which may be associated with a reduced efficiency on the localization of holes around the 2DEG due to the significantly large electric field or to reaching a critical density of electrons at the 2DEG. As mentioned earlier, on the previous works on GaAs/GaAlAs HJs [16–19], the h-2DEG was only observed for magnetic fields larger than a critical value that corresponded to the filling factor ν = 2, which was pointed out as the limit case at which holes are still localized near the 2DEG. In our measurements, we maintained the magnetic field constant at 19 T. However, with increasing bias voltages, the density of electrons accumulated at the 2DEG should increase, and therefore, its filling factor should also increase. Therefore, it is possible that the condition ν ≥ 2 is attained for an applied bias voltage of about 0.5 V, resulting in the fading out of the 2DEG-h transition.
The observed 2DEG-h emission presents a high circular polarization degree with abrupt energy discontinuities after the electron resonance. This effect can be explained considering the increase of electron density in the accumulation-layer after the electron resonance and by changes in the overlap between the 2D electron and 3D hole wave functions induced by magnetic field which affects the 2DEG-h radiative recombination lifetimes of photo-excited holes [18, 19].
In conclusion, we have observed small oscillations on the polarization degree from the QW as a function of the voltage. We have evidence of highly polarized 2DEG and 2DHG in the RTD which can contribute to the polarization degree of carriers in the QW. The voltage dependence of the 2DEG-h emission under magnetic field presents some anomalies which can be explained by the voltage dependence of tunneling dynamics of carriers in the structure. Our results imply that the double-barrier structure creates a polarized two-dimensional gas with a strongly enhanced g-factor, which can act as a spin-polarized source of injected carriers in the structure. However, the circular polarization of carriers in the double-barrier region seems also to depend on various other points, including the g-factors of the different layers, the spin-polarization of carriers in the contact region, the density of carriers along the structure, and the Rashba and Zeeman effects in the valence band.
resonant tunneling diodes
two-dimensional electron gas
two-dimensional hole gas.
The financial support from FAPESP, CAPES, CNPq, and U.K. Engineering and Physical Sciences Research Council and EuroMagNET II is gratefully acknowledged.
- Hanbicki A, Van Erve OMJ, Magno R, Kioseoglou G, Li CH, Jonker BT, Itskos G, Mallory R, Yasar M, Petrou A: Analysis of the transport process providing spin injection through an Fe/AlGaAs Schottky barrier. Appl Phys Lett 2003, 82: 4092. 10.1063/1.1580631View Article
- Jiang X, Wang R, Shelby RM, Macfarlane RM, Bank SR, Harris JS, Parkin SSP: Highly spin-polarized room-temperature tunnel injector for semiconductor spintronics using MgO(100). Phys Rev Lett 2005, 94: 056601. 10.1103/PhysRevLett.94.056601View Article
- Motsnyi VF, Van Dorpe P, Van Roy W, Goovaerts E, Safarov VI, Borghs G, De Boeck J: Optical investigation of electrical spin injection into semiconductors. Phys Rev B 2003, 68: 245319. 10.1103/PhysRevB.68.245319View Article
- Fiederling R, Keim M, Reuscher G, Ossau W, Schmidt G, Waag A, Molenkamp LW: Injection and detection of a spin-polarized current in a light-emitting diode. Nature 1999, 402: 787. 10.1038/45502View Article
- Ohno Y, Young DK, Beschoten B, Matsukura F, Ohno H, Awschalom DD: Electrical spin injection in a ferromagnetic semiconductor heterostructureD. Nature 1999, 402: 790. 10.1038/45509View Article
- Oestreich MJ, Hübner MJ, Hägele D, Klar PJ, Heimbrodt W, Rühle WW, Ashenford DE, Lunn B: Spin injection into semiconductors. Appl Phys Lett 1999, 74: 1251. 10.1063/1.123515View Article
- Jonker BT, Park YD, Bennett BR, Cheong HD, Kioseoglou G, Petrou A: Robust electrical spin injection into a semiconductor heterostructure. Phys Rev B 2000, 62: 8180. 10.1103/PhysRevB.62.8180View Article
- Braden JG, Parker JS, Xiong P, Chun SH, Samarth N: Direct measurement of the spin polarization of the magnetic semiconductor (Ga,Mn)As. Phys Rev Lett 2003, 91: 056602. 10.1103/PhysRevLett.91.056602View Article
- Mattana R, George JM, Jaffres H, Van Dau FN, Fert A, Lepine B, Guivarc'h A, Jezequel G: Electrical detection of spin accumulation in a p-type GaAs quantum well. Phys Rev Lett 2003, 90: 166601. 10.1103/PhysRevLett.90.166601View Article
- Gruber Th, Keim M, Fiederling R, Reuscher G, Ossau W, Schmidt G, Molenkamp LW, Waag A: Electron spin manipulation using semimagnetic resonant tunneling diodes. Appl Phys Lett 2001, 78: 1101. 10.1063/1.1350600View Article
- Slobodskyy A, Gould C, Slobodskyy T, Becker CR, Schmidt G, Molenkamp LW: Voltage-controlled spin selection in a magnetic resonant tunneling diode. Phys Rev Lett 2003, 90: 246601. 10.1103/PhysRevLett.90.246601View Article
- de Carvalho HB, Galvão Gobato Y, Brasil MJSP, Lopez-Richard V, Marques GE, Camps I, Henini M, Eaves L, Hill G: Voltage-controlled hole spin injection in nonmagnetic GaAs/AlAs resonant tunneling structures. Phys Rev B 2006, 73: 155317. 10.1103/PhysRevB.73.155317View Article
- de Carvalho HB, Brasil MJSP, Galvão Gobato Y, Marques GE, Galeti HVA, Henini M, Hill G: Circular polarization from a nonmagnetic p-i-n resonant tunneling diode. Appl Phys Lett 2007, 90: 62120. 10.1063/1.2472522View Article
- dos Santos LF, Galvão Gobato Y, Marques GE, Brasil MJSP, Henini M, Airey R: Light controlled spin polarization in asymmetric n-type resonant tunneling diode. Appl Phys Lett 2007, 91: 073520. 10.1063/1.2772662View Article
- dos Santos LF, Galvão Gobato Y, Marques GE, Brasil MJSP, Henini M, Airey R: Polarization resolved luminescence in asymmetric n-type GaAs/AlGaAs resonant tunneling diodes. Appl Phys Lett 2008, 92: 143505. 10.1063/1.2908867View Article
- Ashkinadze BM, Voznyy V, Cohen E, Ron A, Umansky V: Condensation of bulk excitons on a magnetized two-dimensional electron gas in modulation-doped heterojunctions. Phys Rev B 2002, 65: 073311. 10.1103/PhysRevB.65.073311View Article
- van der Meulen HP, Sarkar D, Calleja JM, Hey R, Friedland KJ, Ploog K: Free versus localized hole magnetophotoluminescence in semiconductor heterojunctions near integer filling factors. Phys Rev B 2004, 70: 155314. 10.1103/PhysRevB.70.155314View Article
- Ashkinadze BM, Linder E, Cohen E, Rudenkov VV, Christianen PCM, Maan JC, Pfeiffer LN: Exciton to two-dimensional electron-hole photoluminescence transitions driven by the quantum Hall effect in photoexcited heterojunctions. Phys Rev B 2005, 72: 075332. 10.1103/PhysRevB.72.075332View Article
- Ashkinadze BM, Cohen E, Rudenkov VV, Christianen PCM, Maan JC, Pfeiffer LN: Transition from two-dimensional electron-hole to geminate-exciton photoluminescence in GaAs/Al x Ga 1-x As heterostructures under a high in-plane magnetic field. Phys Rev B 2007, 76: 075344. 10.1103/PhysRevB.76.075344View Article
- Snelling MJ, Blackwood E, MacDonagh CJ, Harley RT, Foxon CTB: Exciton, heavy-hole, and electron g- factors in type-I GaAs/AlxGa1-xAs quantum-wells. Phys Rev B 1992, 45: 3922. 10.1103/PhysRevB.45.3922View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.